multi-laser diode area melting
White Rose Research Online URL for this paper:
Version: Published Version
Zavala-Arredondo, M., Ali, H., Groom, K.M. et al. (1 more author) (2018) Investigating the
melt pool properties and thermal effects of multi-laser diode area melting. International
Journal of Advanced Manufacturing Technology. ISSN 0268-3768
This article is distributed under the terms of the Creative Commons Attribution (CC BY) licence. This licence allows you to distribute, remix, tweak, and build upon the work, even commercially, as long as you credit the authors for the original work. More information and the full terms of the licence here:
If you consider content in White Rose Research Online to be in breach of UK law, please notify us by
Investigating the melt pool properties and thermal effects of multi-laser
diode area melting
Miguel Zavala-Arredondo1&Haider Ali1&Kristian M. Groom2&Kamran Mumtaz1
Received: 7 February 2018 / Accepted: 16 April 2018
#The Author(s) 2018
Diode area melting (DAM) is a new additive manufacturing process that utilises customised architectural arrays of low-power laser diode emitters for high-speed parallel processing of metallic feedstock. The laser diodes operate at shorter laser wavelengths (808 nm) than conventional SLM fibre lasers (1064 nm) theoretically enabling more efficient energy absorption for specific materials. This investigation presents the first work investigating the melt pool properties and thermal effects of the multi-laser DAM process, modelling generated melt pools the unique thermal profiles created along a powder bed during processing. Using this approach process, optimisation can be improved by analysing this thermal temperature distribution, targeting processing conditions that induce full melting for variable powder layer thicknesses. In this work, the developed thermal model simulates the DAM processing of 316L stainless steel and is validated with experimental trials. The simulation indicates that multi-laser DAM methodology can reduce residual stress formation compared to the single point laser scanning methods used during selective laser melting.
Keywords Diode area melting . Additive manufacturing . Finite element . Cooling rate . Temperature gradient
AM Additive manufacturing SLM Selective laser melting EBM Electron beam melting DAM Diode area melting FEM Finite element model
TGM Temperature gradient mechanism CR Cooling rate
DFLUX Distributed heat flux
MPHF Modified prismatic laser heat flux LBP Laser beam profile
Additive manufacturing (AM) technologies are capable of creating geometrically efficient structures with low material wastage. Laser-based selective laser melting (SLM) and electron-based electron beam melting (EBM) AM systems are increasingly being used in high value sectors to directly manufacture metallic end-use parts from a variety of alloys. During processing, the melting source (deflected laser/ electron beam) selectively scans and melts regions of a pre-deposited powder bed. Cross sections of the part are fused in layers, built up successively to create the complete 3D object. This method of layered fabrication, combined with the high precision of laser melting, allows for a greatly expanded de-sign freedom with minimal feedstock waste.
Diode area melting (DAM) is a novel powder-bed-based AM process for the manufacture of metallic components with ability to process materials with melt temperatures in excess of 1400 °C  using a multi-spot array of low powered laser beams. The DAM heat input mechanism can improve SLM limitations with regard to process thermal evolution, which are known to induce high residual stresses and promote cracking due to the very high cooling rates involved. The thermal * Kamran Mumtaz
Department of Mechanical Engineering, University of Sheffield, Sheffield S1 3JD, UK
2 Department of Electronic & Electrical Engineering, University of
behaviour of DAM is analysed in the present work and com-pared to that of SLM reported in literature.
1.1 State-of-the-art in diode area melting
The DAM methodology replaces the traditional galvo scanning methodology used within single fibre laser SLM systems with multiple non-deflected low power laser diode beams that scan and selectively melt powdered feedstock material in parallel. A multi-layer 4.5 × 4.5 × 6 mm stainless steel sample composed of multiple ~ 150μm layers with areas of cross-sectional micro density comparable to SLM has been reported in . The total laser power and scanning speed used for manufacturing the DAM 3D part were 50 W and 0.5 mm s−1, respectively. Lack
of fusion was observed in regions between layers as well as limited substrate bonding. An energy density 86 J mm−3in
DAM has been theorised as the minimum required for produc-ing high-density parts with penetration depths similar to SLM . In the present work, a finite element model (FEM) capable of simulating the DAM process is used for analysing the cooling rate and temperature gradient mechanisms that describe the DAM thermal evolution. The model was able to predict melt-pool dimensions within 91–94% accuracy. FEM-assisted parameter optimisation was used to compare the DAM thermal evolution with that of SLM for the same material. The FEM predicted DAM cooling rate and temperature gradient similar to those of optimised SLM methodologies with lower residual stress formation.
1.2 Residual stresses in selective laser melting (SLM)
The rapid melting and solidification mechanisms during SLM lead to very high-temperature gradients that result in high re-sidual stress formation . The nature and origins of residual stresses in laser processes such as SLM are described in . These can be either mechanical, thermal or plastic and can be typified by the dimensional scale that better describes the prop-erty under consideration. Three types of residual stresses are characterised in , denominated as Types I, II and III. Typically, Type I residual stress scale is used to characterise the SLM mechanism since it varies over large distances similar to the dimensions of the additively manufactured part. Residual stresses in SLM are unwanted since they can reduce the toler-ance of the as-built part to an external applied force and cause part deformation when removed from the substrate. Moreover, residual stresses can reduce the strength of the part and promote the propagation of cracks from the surface. Laser-based pro-cesses are known to result in high levels of residual stresses due to the large thermal gradients inherent to the rapid melting-solidification mechanism. In , the temperature gra-dient mechanism (TGM) is described which causes residual stresses in sheet metal plates during laser heating and cooling phases as illustrated in Fig. 1. High-temperature gradients
develop due to the rapid heating of the upper sheet surface and the comparatively slow heat conduction through the lower surface. The laser-heated surface experiences a thermal expan-sion which is restricted by the underlying solid material induc-ing elastic compressive strains. The laser-heated surface is plas-tically compressed when the material’s yield strength is reached causing in turn bending away from the laser beam. A counter bending occurs during the cooling phase due to the thermal contraction of the cooling surface. In SLM, the bending and counter bending mechanisms are inhibited by the underlying solid material (i.e. solid substrate and/or previously solidified layers). During the cool-down phase, shrinkage of the thermally contracted top layers is inhibited resulting in tensile stresses in the added top layer and compressive stress below. In , it was concluded that it is possible to reduce residual stresses by (1) applying heat treatment using the laser source and/or (2) reduc-ing temperature gradients by heatreduc-ing the substrate plate.
1.3 Temperature gradients and cooling rate
in selective laser melting (SLM)
The temperature gradients and cooling rate along thex,yand z-directions during SLM of stainless steel have been modelled in . The model was validated with experimental tests. Figure2shows the cooling rate of five scan tracks in (a) the x-yplane at top surface of the powder bed and (b) they-zplane along the cross-section (A-A′) at the centre of the processing region of a typical SLM scanning strategy. Figure2c, d shows the thermal history of Point A3, in Fig.2a, and the temperature distribution in the z-direction, respectively. The process pa-rameters used in Fig.2a–d are laser power 120 W, laser diam-eter 140μm, hatch spacing 65μm, layer thickness 50μm and scanning speed 715 mm s−1. It can be seen in Fig. 2a that
This explains the higher temperature gradients along the scan-ning direction compared to those perpendicular as reported in . Cooling rates can be observed to reduce steeply along the cross sectionA-A′during tracks 1 and 2, reaching stable levels in Points A3 to A5, in Fig.2a. Starting from track 3, an in-variance in the cooling rates across laser tracks is shown, which is also depicted in Fig.2b by a constant melt depth after track 3. The melt depth and cooling rate invariance are expect-ed to continue if more tracks are analysexpect-ed. The thermal history of point A3 is plotted in Fig.2c. Here, several temperature peaks are observed due to accumulation of subsequent laser tracks. Two lower secondary peaks (first and last in Fig.2c) can reach melting temperatures before and after the main melt-ing peak respectively, inducmelt-ing localised laser heat treatment. The cooling rate can be obtained from Eq.1,
Cooling rate °Cs−1¼ΔT Δt
ð Þ−Tsolidusð Þ°C
tliquidusð Þs−tsolidusð Þs
where Tliquidus= 1425 °C and Tsolidus= 1385 °C for
stain-less steel . The cooling rates of the three temperature peaks observed in Fig. 2c are 2.08E + 05 (°C s−1),
1.07E + 05 (°C s−1) and 1.51E + 05 (°C s−1) for the first,
main and last peak, respectively. In Fig. 2d, the slope of the temperature distribution curve in the z-direction be-comes steeper as z increases, which is an indication of increasing temperature gradient and cooling rate when distance into the substrate (or previously solidified layers) is increased. The instant temperature gradient from the top surface of the substrate to the melt depth is |ΔT/Δz| (top surface to melt depth)= 11.16 °C μm−1.
A comparison of Fig.2a, b shows that cooling rates tend to be higher at the intersection with the substrate (Fig.2b) than at the top surface of the process layer (Fig.2a). This is in agree-ment with the study conducted in  who evaluated the residual stress distribution of a stainless steel sample along the z-direction. Figure3 shows the residual stresses curve profile for central regions of a 3 × 3 cm SLM one-layer samples.
Fig. 2 Cooling rate in theax-yplane at the top surface of the powder bed
andby-zplane along the cross sectionA-A′.cThermal history of point A3
andbinstant temperature distribution inz-direction for laser power
120 W, hatch spacing 65μm, layer thickness 50μm and scan speed 715 mm s−1. Adapted from 
The parameters used in Fig.3were laser power 50 W, laser diameter 70μm, hatch spacing 60μm, layer thickness 50μm and scanning speed 100 mm s−1. Figure3shows that residual
stresses tend to be higher in regions closer to the substrate surface. Also, Fig.3shows higher levels of residual stresses along the scanning direction than those perpendicular to the scanning vectors. It can be concluded that cooling rates and residual stresses are directly correlated as the distribution of the highest cooling rates shown in Fig.2a, b are represented by the highest levels of residual stresses in Fig.3.
The microstructure of the material can be an indication of the mechanical properties of the part. For instance, hardness can increase if grain size is reduced. Fine microstructures are typical of laser-based processes due to their characteristic rapid cooling. Rapid solidification processes such as SLM can have cooling rates ranging from 103to 107. The higher the cooling rate, the higher the material hardness. However, too high cooling rates may promote cracking in brittle materials. The primary dendrite arm spacingλof stainless steel components can be
used to characterise grain size as described in Eq.2.
λ1ðμmÞ ¼80ðCRÞ−0:33 ð2Þ
where CR refers to the cooling rate in K s−1or °C s−1. The
relation of primary dendrite arm spacingλ1with grain size is
defined in . Typical cooling rates in SLM of stainless steel
can be on the order of magnitude ~ 105to ~ 106°C s−1as
reported in , which result in cell spacing ranging fromλ1
= ~ 0.84–1.79μm. Such values are characteristic of very fine microstructures typical of extremely hard components that can be susceptible to cracking.
1.4 Mechanisms for reducing residual stress build-up
In Sect.1.2, the mechanisms for reducing residual stress build-up have been presented, namely (1) applying heat treatment using the laser source and (2) heating the substrate plate. These mechanisms are typically used for reducing thermal gradients and cooling rates in SLM. In  (see Sect.1.3) it is shown that processing with ~ 50% scan-tracks overlap (hatch spacing < laser diameter) can induce up to three tem-perature peaks above the melting point of the process material which might result in selective re-melting of regions exhibiting cooling rate invariance (see Fig.2a, b). A similar behaviour was observed when using hatch spacing equal to laser diameter in . However, when processing with hatch spacing > laser diameter, no selective re-melting occurred. Selective re-melting can be scaled-up to the whole bed by using re-scanning strategies (i.e. re-melting by scanning the process layer multiple times). Re-scanning strategies together with substrate pre-heating were used in  to produce high-density stainless steel SLM parts by reducing thermal gradi-ents and cooling rates. They observed a strong influence of these parameters on the properties of the as-built part. It was observed that the highest pre-heating temperature tested (200 °C) + re-scanning resulted in samples with lower surface roughness and higher density. However, re-scanning by itself (i.e. without the assistance of substrate pre-heating) induced more cracks due to the formation of brittle martensite phase promoted by the higher cooling rates. Re-melting every layer can thus induce very high residual stress build-up and lead to cracking. It was concluded that lowering the thermal gradients and cooling rates by pre-heating the substrate can promote less martensite formation which can in turn reduce the thermal stresses and the amount of cracking. Moreover, in , it was reported that higher pre-heating temperatures can completely alleviate residual stresses by effectively minimising cooling rates and temperature gradients.
Fig. 3 Residual stress curve profile for central regions of a 3 × 3 cm one-layer sample. Adapted from 
1.5 Melt-pool penetration into substrate
In SLM, penetration of the melt-pool into the substrate allows for deposition of further layers without removing the previously melted layer, while the wiper moves along the substrate. A density analysis for SLM processing of 316L stainless steel was performed in  in order to iden-tify the optimum process parameters for achieving > 99% part’s density. A range of laser powers (250–400 W) and scan speeds (1500–1900 mm s−1) were investigated,
resulting in substrate penetration depths ranging from ~ 65 to ~105μm. Such penetration depths allow re-melting of previously processed layers (n.b. typical layer thickness in SLM can be 50μm) which facilitates the formation of an even surface. When the surface is even, the powder distri-bution of the next layer will be more homogenous and will reduce the entrapment of air . This can reduce porosity and improve the density of the part. Such penetration depths are therefore a requirement for high density in DAM components.
2 Modelling the diode area melting process
An isotropic enhanced thermal conductivity model has been adapted from the model developed in  to simulate DAM processing of 316L stainless steel powder. The mod-el takes into account the DAM Laser Beam Profiles (LBPs) and process parameters (i.e. laser power and scan speed) presented in the DAM experimental investigation conduct-ed in . The non-linearity of temperature-dependant ma-terial properties and phase changes is also considered. The modelling approach used in the present work is based upon the concept of a moving volumetric heat source (typically used in SLM modelling ) with enhanced penetration
depth, combined with enhanced thermal conductivity through the substrate and the surrounding powder to im-prove computational efficiency, as described in . The aim of the present work is to simulate the DAM process using optimised conditions that enable process energy den-sity of 86 J mm−3, which has been theorised as the
mini-mum required for processing fully dense multi-layer parts in the densification analysis conducted in . The cooling rates, thermal distribution and temperature gradients of DAM are contrasted with those of SLM in order to com-pare the two different heat input mechanisms.
2.1 Laser heat source modelling
An ABAQUS DFLUX (Distributed Heat Flux) subroutine written in FORTRAN was used to simulate the laser as a moving volumetric heat source. This approach was used to account for the laser penetration effect into the powder, which according to  is 120 μm for stainless steel 316L powder. To make the simulation more efficient, the volumetric heat source was applied to a 260μm-thick layer of powder, as used in the DAM densification analysis con-ducted in , along with a 250μm depth into the substrate . A Modified Prismatic laser Heat Flux (MPHF) model, similar to the cylindrical representation model explained in [19, 20], was used in the present work to represent the variation of radial laser intensity. Equation 3 shows the MPHF model, describing the heat flux of the rectangular multi-beam laser output typical of the DAM process,
qmod prism Wmm−2¼0:864αP
wherePis the laser power in W, andb andhare the base and height of the rectangular-shaped multi-beam laser di-ode irradiation on the powder bed top surface. From the DAM laser beam profiles (LBPs) described in , these are b= 4.75 mm andh= 0.25 mm for LBP1,b= 6.5 mm and h= 0.3 mm for LBP2 andb= 9.4 mm andh= 0.4 mm for LBP3 (Fig. 4). α is the laser absorptivity value for the
316L stainless steel powder bed. An absorption coefficient
α= 0.5 was used for the present work as used in . The
LBPs shown in Fig.4 are top powder-bed views obtained
Substrate 2 mm
260 µm 20 µm
increasing to 500 µm downward
125 µm square
20 µm x 13 elements
b ( )
Fig. 5 aModel andbmesh dimensions. DimensionLvaries fromL= 6 mm for LBP1 toL= 10 mm for both LBP2 and LBP3
Table 1 Thermal properties of process 316L stainless steel powder and mild steel substrate 
Material Latent heat (mJ t−1)
Solidus temperature (°C)
Liquidus temperature (°C)
using a Spiricon camera-based beam profiler, and an opal glass target as described in  and the beam dimensions were measured using Ophir BeamMic software. It can be seen that the power distribution tends to be flatter whilst reducing beam dimensions (i.e. reducing individual spot size and spot period). LBP1 showed a typical flat-top laser profile with a homogeneous power distribution across the length of the profile. Equation4 shows the laser intensity in the radial direction Ir (W mm−2) used in the present
¼cf⋅qmod prism ð4Þ
wherecfis the correction factor required for achieving melt
pool size and temperature distribution in good agreement with published results.cfwas calculated through FEM
tri-als for different process parameters. The laser intensity in the melt depth direction, described byIz(mm−1), has been
modelled as a parabolic relation as presented in . Equation 5 shows the heat flux definition that describes the moving heat source simulation used in the present work,
˙ Wmm−3¼ I
ð Þ ð5Þ
2.2 Simulation model
A simulation model consisting of a single 260μm layer of 316L stainless steel powder deposited upon a 2 mm thick mild steel substrate is presented in this work. The dimensions of the simulated substrate vary with the different LBPs modelled and range from 6 × 2 × 2 mm for LBP1 simulation to 10 × 2 × 2 mm for both LBP2 and LBP3 simulation (Fig. 5a). A 1.2 mm-length track (moving along they-direction) was ob-served to result in a penetration depth invariance as described in Sect.1.3, Fig.2b. The solidification behaviour and cooling rate are expected to remain constant if a longer track is analysed. Therefore, a 1.2 mm scan was used to simulate the DAM process. Numerical simulation is carried out using the ABAQUS finite element package. Mesh element type DC3D8 (i.e. 8-node linear heat transfer brick element) was used. Figure5b shows the 125 × 125 × 20 μm mesh size used for the powder layer. The layer is composed of 13 elements in the z-direction to create the 260μm layer thickness. The substrate mesh was biased to move from 20μm at the top, increasing to 500μm at the bottom in order to keep the number of mesh elements to a minimum and reduce the model size and com-pilation time. The initial temperature of the substrate is 25 °C. The rectangular heat source dimensions on the top surface of the powder bed vary with respect to the different beam profile dimensions (i.e. LBP1, LBP2 and LBP3), as described in Sect.2.1. The nodal temperatures are monitored in time steps to determine material phase changes. The material properties are updated for the appropriate elements/nodes (interpolating when necessary) as the laser moves continuously along the simulated region (i.e. scanned track) until the whole defined geometry has been analysed. The material properties used in the model are summarised in Table1. Temperature-dependent properties are detailed in .
2.3 Correction factor for varying parameters
To simulate the DAM melting process, multiple FE iterations were undertaken in order to identify the appropriate correction factor cf described in Sect. 2.1, for the different process
Fig. 6 Factorcffor varyingalaser
power andbtotal melting/beam area (i.e. varying LBPs). Melting/ beam area inawas 1.19 mm2
(LBP1), and a range of scanning velocities was used (i.e. 1, 3 and 5 mm s−1). Laser power and scan
speed inbwere fixed to 50 W and
5 mm s−1, respectively
Fig. 7 Experimental and simulated melt depth dimensions for the different laser beam profiles LBP1–3. Laser power and scan speed remained constant at 50 W and 5 mm s−1, respectively. Each LBP was
simulated using the correspondingcffrom Fig.6b where LBP1, 2 and 3
parameters (i.e. laser power, scan speed and melting area). The iterations were conducted until the modelled melt dimensions approached the geometrical data experimentally acquired in literature, to the minimum % error possible. Therefore,cfhas
to be considered as a boundary condition in the present DAM FEM. It was observed that laser power and beam dimension (i.e. melting area of a given LBP) were the only parameters definingcf. Scan speed was observed to have a negligible
effect in determiningcf. Therefore,cf remained constant at
varying scan speeds for a given laser power and LBP. Figure6a plots the chosencffor varying laser power (i.e. 30,
40 and 50 W) and scanning velocities (i.e. 1, 3 and 5 mm s−1)
at constant LBP1 with a melting area of 1.19 mm2. Figure6b plots the chosencffor varying melting area (i.e. 1.19, 1.95 and
3.76 mm3for LBP1, LBP2 and LBP3, respectively) at con-stant 50 W and 5 mm s−1. Trend lines are fitted for both plots,
allowing extraction ofcffor process optimisation (i.e. using
higher laser power and smaller melting area). The equations shown in Fig.6a, b that describe the effect of laser power and melting area, respectively, were used to extractcffor the
pro-cess optimisation model.
3 Model validation
In order to determine the suitability of the FEM for predicting temperature evolution in DAM of stainless steel 316L, a com-parative study with the experimental work reported in  was conducted. The simulated melt-pool dimensions were com-pared with the experimental observations published in ,
for a range of process parameters. The simulated temperature evolution was determined by measuring the nodal thermal history of defined points when irradiated by the moving laser heat source. The present section details the validation of the SLM model adapted for DAM simulation.
3.1 Melt-pool dimensions
In the present section, experimental melt-pool dimensions are compared with simulated values using the corresponding cf
described in Fig.6. Figure7shows the measured and simu-lated melt depths for varying laser melting/beam areas (LBP1–3) at constant 50 W and 5 mm s−1. It is assumed that
thecftrend as a function of melting area (see Fig.6b) is the
same at any constant power and speed. It was reported in  that LBP1 showed the more consistent results when varying energy density parameters (i.e. laser power and scan speed). Several failed samples were reported using lower energy den-sity levels with LBP2 and 3. Therefore, only LBP1 were modelled for varying laser power and scan speed.
Figure8 shows the measured and simulated melt dimen-sions for LBP1. Figure8a compares the average experimental and simulated melt depths as a function of laser power and scan speed. Figure 8b shows a comparison of experimental melt widths against the simulated values for varying laser power and scan speed. Good agreement between experimental findings and simulated values of melt dimensions (i.e. melt depth and width) for varying parameters (i.e. laser power, scan speed and melting/beam area) was observed. Figure9shows an example of the experimentally measured melt dimensions Fig. 8 Experimental and simulatedamelt-depth andbmelt-width dimensions for LBP1, varying laser power and scan speed. Each combination of
parameters was simulated using the correspondingcffrom Fig.6a for the different laser powers
5.067 mm 0.244 mm
Non-melted powder Melted and
Fig. 9 aExperimentally
measured melt dimensions for 316L stainless steel powder processed from 260μm layer thickness with 42 J mm−3energy
(Fig.9a) together with the modelled melt dimensions (Fig.9b) using the DAM process parameters (50 W power and 1 mm s−1scan speed) that resulted in the highest part density
(99.68% sectional micro density and 87.29% cross-sectional macro density) from the parametric investigation conducted in . The experimentally acquired melt dimen-sions of 5.067 × 0.244 mm are in good agreement with the FEM simulated dimensions of 4.766 × 0.222 mm. The pre-dicted melt-width is ~ 6% less than the average experimentally measured, and the predicted melt depth is 9% less than the average experimentally measured.
3.2 Thermal evolution and maximum temperature
The thermal history predicted by the FEM has been compared to the experimentally acquired temperature evolution in  (details of the equipment used, temporal and geometrical res-olution, etc. used to record the experimentally acquired tem-perature fields can be found in ). The temperature transient was measured from the top surface of the powder bed (XY-plane) for a range of scan speeds with 50 W laser power across the irradiating laser stripe. Due to image saturation, the exper-imentally acquired temperature range was limited to a maxi-mum measured temperature of 1350 °C. The nodal thermal history of a single central point across the beam spatial distri-bution is compared to the experimental data within the mea-sured temperature range. Figure10shows this comparison for the three different scan speeds (5, 3 and 1 mm s−1) investigated
in . It can be seen in Fig. 10a–c that temperature rises steeply up to ~ 1250 °C for all the scan speeds studied, before appearing to saturate to higher temperatures. Better agreement between simulated and experimental data is observed at slower scan speeds (i.e. higher energy density). However, no significant difference was observed when varying scan speed from 3 to 1 mm s−1both in the experimental and the modelled
temperature evolution. From the FEM simulation, the maxi-mum predicted temperatures for the different scanning speeds were 1510, 1519 and 1565 °C for 5, 3 and 1 mm s−1,
respec-tively. Figure11shows the maximum temperatures and the nodal thermal evolution predicted by the FEM for the different scan speeds investigated. Cooling rates were observed to
decrease significantly for slower scan speeds. Temperatures in excess of 1350 °C could not be experimentally measured. However, density analysis conducted in  indicated that melting was achieved, exceeding the melting temperature of stainless steel powder (1450 °C) without reaching too high temperatures that may have caused boiling. The results pre-sented in Figs.10 and11 show that the thermal evolution, temperature trend and maximum temperatures predicted by the FEM agree well with the experimental data. It can be assumed that accurate predictions of the cooling rate and tem-perature gradients can be modelled, which might provide in-sight into the residual stress build-up.
4 Results and discussion
The present section describes the effect of layer thickness in DAM. Also presented is the process optimisation methodolo-gy, using the correction factor derived from equations in Figs.6a, b. DAM modelling and simulation have been used to investigate the cooling rates and temperature gradients in-herent to the process. Finally, the DAM optimised model is compared with SLM cooling rate, temperature gradient and penetration depth into substrate.
4.1 Effect of layer thickness
In order to investigate the effect of layer thickness, the model was adapted to model 200 and 150μm layer thicknesses. For this, 10 × 20μm elements and 8 × 18.75μm elements in thez -axis (layer depth) were used to model 200 and 150μm layer thickness, respectively. Figure12shows cross-sectional views of the temperature distribution for the 200 and 150μm layer thicknesses modelled at 50 W laser power and 1 mm s−1scan
speed. As described in Sect.3.2, no significant difference in the process thermal evolution was observed when reducing scan speed below 3 mm s−1. Therefore, it can be assumed that
the scan speed 1 mm s−1modelled can be a good
representa-tion of the thermal history of 0.5 mm s−1scan speed reported
excess of the 316L stainless steel melting point (1450 °C) can be achieved uniformly across the scanning direction. In con-trast, the melting temperature could not be reached when sim-ulating the processing of 150μm layer thickness (Fig.12b). In this case, the laser-induced heat irradiated at the top surface of the powder bed rapidly dissipated into the solid substrate, which prevented reaching the melting point. When using 150μm layer thickness, the high thermal conductivity of the solid substrate had a stronger influence on the temperature distribution. For the thicker 200μm layer, lower thermal con-ductivity within the powder bed prevented such rapid heat-sinking into the substrate and better maintained the tempera-ture distribution within the laser-irradiated bed, allowing tem-peratures in excess of 1450 °C to be reached. The aforemen-tioned stainless steel DAM 3D part was processed at 50 W and 0.5 mm s−1. However, a heat dissipation mechanism similar to
that described here, and shown in Fig. 12b, may have prevented good inter-layer bonding in specific and random locations of non-uniform layer thickness.
4.2 Process optimisation
A minimum energy density of 86 J mm−3 is suggested in
literature for manufacturing high-density 3D DAM parts and achieving substrate bonding. Equation6 shows that energy density is directly proportional to laser power and indirectly proportional to beam size and scan speed.
Energy density J mm3
¼ total laser power Wð Þ
total beam area mmð 2Þ scan speed mm
Therefore, higher energy densities can be attained by in-creasing laser power, reducing melting area and/or reducing the scan speed. The total processing time depends directly on scan speed; therefore, increasing scanning velocity is desirable for DAM optimisation, which in turn requires an increase in laser power and/or a decrease in melting area. An increase in total laser power can be achieved by multiplexing the output from multiple laser diode bars resulting in 100 W total laser power. Optimisation of the beam delivery system (by varying collimators and focusing lenses’focal length) can reduce the total melting/beam area by reducing individual beam
Fig. 12 Cross-section images of the FEM showing temperature distribution fora200 andb
150μm layer thickness with LBP1, 50 W and 1 mm s−1
(42 J mm−3energy density)
Fig. 11 Simulated nodal temperature transient for a range of scan speeds at 50 W and LBP1. Maximum simulated temperatures are 1510, 1519 and 1565 °C for 5, 3 and 1 mm s−1, respectively
Table 2 Parameters used for DAM optimisation
Total laser power 100 W
Scan speed 6.12 mm s−1
Energy density 86 J mm−3
Individual laser diameter 100μm Spot period (hatching space) 100μm
dimensions and spots period. A DAM optical configuration composed by an array of multiple 100μm diameter beams (i.e. typical laser dimension in SLM) has been modelled. The theoretically optimised optical configuration model ac-counts for the effect of × 19 individual melting spots, provid-ing a total beam areaA= 1.9 mm × 0.1 mm = 0.19 mm2 con-sidering scan spacing = individual spot diameter (as identified in Sect.1.4 to be the minimum condition for selective re-melting in SLM), with a flat-top laser intensity profile similar to that shown by LBP1 in Fig.4a. The fit to the data shown in Fig.6b describes thecftrend in terms of total melting/beam
area. For the optimisedA= 0.19 mm2, a factorcf= 18.12 has
been calculated using this equation. A difference of 5.82 re-sulted from comparing thecfof the optimised total melting/
beam area (i.e. 0.19 mm2) with that of LBP1 (i.e. 1.19 mm2), as was used in thecftrend analysis shown in Fig.6a. Thecf
trend for varying laser power is described by the equation describing the fit to the data in Fig.6a. Thecffor the optimised
model, increasing laser power to 100 W and using constant total melting/beam areaA= 0.19 mm2, can be calculated using Eq.7.
cf ¼50:436⋅EXPð−0:029⋅PÞ þ5:82 ð7Þ
wherePis laser power in W, althoughcfis dimensionless.
Table2 shows the parameters used in the optimised DAM model.
A 50μm layer thickness, as is typical in SLM, was con-sidered in the process optimisation model. To account for the optimised 100μm single spot size and 50μm layer thickness, the powder bed was adapted to 125 × 50μm in the XY plane withL= 6 mm (see Fig.5a) and 16.667μm × 3 elements in thez-direction.
4.3 Thermal spatial distribution
The modelled temperature distribution of the top surface of the powder bed along the scanning direction is shown in Fig. 13 for the DAM optimised configuration. The instant temperature of 15 nodes/points, 700 μm along the scanned track (as detailed in Fig.13), has been extracted in order to plot the predicted thermal distribution along the scanning di-rection. Maximum temperature 1851 °C has been predicted (see nodal temperature label in Fig.13). Figure14shows the extracted spatial thermal distribution that describes the instant nodal temperature along the 700μm in they-axis (composed by the 15 data points/nodes) described in Fig.13for the DAM optimisation mechanism. The melting-solidification range shown in Fig. 14is delimited by the solidus and liquidus temperatures of the powder (1385 and 1425 °C, respectively). The peak of the curve in Fig.14(i.e. maximum temperature) represents the melt-pool centre which is located at the plotted distance of 525μm. It can be seen that the melt pool starts solidifying 150μm behind the melt-pool centre in the scan-ning direction. The DAM s/d ratio along the scanscan-ning direc-tion can be s/d = 0.08 (i.e. 0.15 mm solidificadirec-tion distance / 1.9 mm total multimode beam diameter). This will lead to significant reduction of the temperature gradient in DAM compared to SLM, which ultimately can result in reduced residual stress build-up.
Figure15shows the simulated temperature distribution and material solidification evolution of parts processed using the DAM optimisation mechanism in a range of views (plan, front and side cross-sections, and a dimensioned isometric view). Figure15a shows the temperature distribution in the XY-plane (plan view) along the scanning direction. This takes the form of a uniform, non-elongated elliptical temperature distribu-tion, which is expected from using a parallel multi-beam melt-ing scheme and slow scannmelt-ing velocities, and differs to the elongated-tail-shape temperature distribution with high-Fig. 13 Simulated temperature
distribution at the top surface of the powder bed, along the scanning direction using optimised DAM configuration with 100 W and 6.12 mm s−1. The
red spots show the location of the 15 nodes/points along 700μm in the scanning direction for nodal temperature measurement
temperature gradients typical of SLM. The uniformity of the DAM temperature distribution reduces the temperature gradi-ents along and across the scanning direction, resulting in lower heating and cooling rates. Figure15b shows a dimensioned isometric view with scanning direction and the region used for volumetric heat addition. Figure15c, d shows the temperature distribution in the XZ-plane (front view) and YZ-plane (side view) across and along the scanning direction, respectively. Uniform temperature distribution similar to that within the top surface can be observed in Figs.15c, d, which might be evi-dence of uniform cooling rates and temperature gradients in all directions. The low-temperature gradient across and along the melt-pool depth in both the front and side view would lead to reduced contraction upon cooling, controlling the residual stress development as described by the temperature gradient mechanism and cool-down phase model presented in Sect.1.2.
4.4 Cooling rate and temperature gradient
The correlation between temperature gradients and residual stress build-up in SLM has been previously described in Sect. 1.3. Low-temperature gradients inherent in the DAM process may also result in low residual stress build-up. In the DAM-optimised mechanism, the 100 μm scan intervals are composed by overlapping 100μm laser spots, similar to the selective re-melting SLM mechanism described in Sect.1.4
for hatch spacing = laser diameter. Figure16a shows a typical SLM scanning strategy compared to that of DAM in Fig.16b. The temperature evolution at the top surface of the powder bed in points A (similar to point A3 in Fig.2a) and B for SLM Fig. 15 a(Plan view) Simulated temperature and material solidification
evolution along the scanning direction in XY-plane.bDimensioned
isometric view showing the depth used for volumetric heat addition.c
(Front view) Temperature and material solidification evolution across the
depth of the scanning direction in XZ-plane.d(Side view) Temperature
and material solidification evolution along the depth of the scanning direction in YZ-plane.
Fig. 17 Simulated DAM nodal thermal evolution of point B (in Fig.16b) along the scanning direction
Fig. 16 aTypical SLM scanning strategy of a single raster scan vector.b
and DAM, respectively, is compared in this section. Point A was selected since a stable melt depth and invariant cooling rate was observed as described in Sect. 1.3and Fig. 2a. A similar behaviour was observed at point B in the DAM model. The scan interval (i.e. hatch distance in SLM) and distance between spots (i.e. spot period in DAM) for both SLM and DAM are 65 and 100μm, respectively.
The thermal history of points A and B is analysed in order to compare their correspondent cooling rates. Point A is equiv-alent to point A3 in Fig.2a in which thermal history is plotted in Fig.2c. As mentioned before in Sect.1.3, point A can be subjected to three peak melting temperatures with 2.08E + 05, 1.07E + 05 and 1.51E + 05 °C s−1cooling rate values,
respec-tively. The simulated thermal history of point B (Fig.16b) has been extracted from the optimised DAM model and is plotted in Fig.17. Here, a DAM cooling rate 8.61E + 03 °C s−1can be
calculated using Eq.1, which can result in coarser microstruc-tures than SLM, with λ1= 4, from Eq.2. However, DAM
cooling rates on the order of magnitude 103are in the lower limit of typical values for rapid-solidification processing. Therefore, it is concluded that DAM can benefit from the superior mechanical properties that characterises rapid cooling mechanisms while exhibiting cooling rates low enough to avoid cracking.
Figure18a shows the simulated depth-resolved temperature gradient for the DAM optimisation model, plotting the temper-ature at the top surface of the melt pool as well as 190 and 380μm below the top surface of the melt-pool. These points are highlighted in the cross-section view of the model pictured in Fig.18b. The equation shown in Fig.18a describes the tem-perature distribution in the z-direction. It has been used for comparing the thermal distribution of DAM with that of SLM shown in Fig.2d in thez-direction. A 132μm penetration into substrate is predicted by the DAM model. Therefore, Δz(top
surface to melt depth) is 132 μm + 50 μm layer thickness =
182μm. ΔT(top surface to melt depth)can be obtained using the
equation in Fig.18to calculate temperature at a givenzlocation (where z= 0 represents the top surface), which gives |ΔT/
Δz|(top surface to melt depth)= 1.65 °Cμm−1for DAM compared
to the 11.16 °Cμm−1of SLM reported in Sect.1.3. Therefore,
the temperature gradients at the junction of the powder layer with the substrate (i.e. where the highest residual stresses are expected to develop) can be 11.16 / 1.65 = ~ 6.8 times lower than SLM, which might result in a proportional reduction of residual stress formation. From Fig.3, it can be assumed that the maximum levels of residual stresses ~ 350 MPa perpendic-ular and ~ 450 MPa parallel to the scanning direction of a one-layer part, typical in SLM of stainless steel, can be reduced to ~ Fig. 18 aTemperature gradient
prediction of the DAM optimised mechanism between the top surface of the melt, 190 and 380μm below the melt-pool from FE simulation for DAM of 316L stainless steel one-layer components.bCross-sectional
view of the model showing the top, 190 and 380μm position considered for temperature gradient estimation
Powder melted and solidified
into substrateFig. 19 Cross-view of the
50 and ~ 70 MPa, respectively, with ~ 6.8 lower temperature gradients, which can be characteristic of the DAM process.
4.5 Melt-pool penetration into substrate
Figure19shows a cross-sectional view of the simulated DAM penetration depth into substrate, using the optimised model.
The area in red represents the phase changes (i.e. powder-to-liquid-to-solid) of the laser-scanned layer of powder that was melted and solidified. The areas in blue represent the surrounding powder that was not scanned/melted by the laser. The simulated penetration depth of the DAM process is 132μm, which is comparable to that reported in literature for the same material. Higher melt depths in SLM are known to result from decreasing scanning velocities. Similarly, higher DAM penetration depths may be the result of the slower scan-ning speeds compared to SLM.
The computational efficiency of the adapted modelling ap-proach for SLM simulation has proven to be applicable for DAM simulation using the appropriate boundary conditions. Melt-pool dimensions and thermal evolution with high corre-lation with published experimental results validated the modelling approach presented. The model was capable of predicting temperature evolution through the powder layer to the solid substrate, modelling the DAM limitation of inter-layer melt disruption reported in literature for processing multi-layer 316L stainless steel components. A DAM config-uration with optimised energy density parameters has been modelled with 100μm individual laser diameter, 100μm spot period (i.e. hatch spacing), 100 W total laser power and 6.12 mm s−1 scan speed. The optimised energy density
modelled has been compared with SLM for the same process material. It was observed that the DAM methodology can effectively reduce temperature gradient and cooling rates, the-oretically reducing residual stress build-up due to its charac-teristic melting mechanism composed of multiple parallel scanning vectors with low individual power and low scan speeds. The analysis concludes that the predicted temperature gradients and cooling rates of DAM can match those of optimised pre-heated SLM mechanisms (either by selective re-melting, substrate pre-heating or both). It was observed that the melt-pool penetration depth in DAM of 316L stainless steel can be similar to values typical of SLM for the same process material. The present work analysed the thermal be-haviour of a multi-beam array of low power lasers in additive manufacturing. The authors suggest that the DAM technique can significantly reduce temperature gradients and cooling rates of a laser-based additive manufacturing process, resulting in complete alleviation of residual stresses. The
thermal analysis described in the present work can be used to compare DAM with SLM in terms of mechanical behav-iour, microstructure and residual stresses of as-built compo-nents in future work.
Acknowledgements The authors would like to acknowledge support from a UK Engineering & Physical Sciences Research Council (EP/ K503812/1) IIKE Proof of Concept award and the Future Manufacturing Hub in Manufacture using Advanced Powder Processes (MAPP) (EP/P006566/1). Also acknowledge support from the Science and Technology National Council (CONACYT) of Mexico.
Open Access This article is distributed under the terms of the Creative
C o m m o n s A t t r i b u t i o n 4 . 0 I n t e r n a t i o n a l L i c e n s e ( h t t p : / / creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appro-priate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Publisher’s NoteSpringer Nature remains neutral with regard to jurisdic-tional claims in published maps and institujurisdic-tional affiliations.
1. Zavala-Arredondo M, Boone N, Willmott J, Childs DTD, Ivanov P, Groom KM, Mumtaz K (2017) Laser diode area melting for high speed additive manufacturing of metallic components. Mater Des 117:305–315
2. Zavala-Arredondo M, Groom KM, and Mumtaz K (2017) Diode area melting single-layer parametric analysis of 316L stainless steel powder. Int J Adv Manuf Technol 1–14
3. Casavola C, Campanelli L, and Pappalettere C (2008) Experimental analysis of residual stresses in the selective laser melting process. in Proceedings of the XIth International Congress and Exposition 3: 1479–1486
4. Withers PJ, Bhadeshia HKDH (2001) Residual stress. Part 2— na-ture and origins. Mater Sci Technol 17(4):366–375
5. Mercelis P, Kruth J, Kruth J-P (2006) Residual stresses in selective laser sintering and selective laser melting. Rapid Prototyp J 12(3): 254–265
6. Li L, Lough C, Replogle A, Bristow D, Landers R, and Kinzel E (2017) Thermal modeling of 304L stainless steel selective laser melting, in Solid Freedorm fabrication, pp 1068–1081
7. Ali H (2017) Evolution of residual stress in Ti6Al4V components fabricated using selective laser melting
8. Smurov IY, Dubenskaya MA, Zhirnov IV, Teleshevskii VI (2016) Determination of the true temperature during selective laser melting of metal powders based on measurements with an infrared camera. Meas Tech 59(9):971–974
9. Mills KC (2002) Recommended values of thermophysical proper-ties for selected commercial alloys. Woodhead
10. Yadroitsev I, Yadroitsava I (2015) Evaluation of residual stress in stainless steel 316L and Ti6Al4V samples produced by selective laser melting. Virtual Phys Prototyp 10(2):67–76
11. Elmer JW, Allen SM, Eagar TW (1989) Microstructural develop-ment during solidification of stainless steel alloys. Metall Trans A 20(10):2117–2131
13. Kempen K, Vrancken B, Thijs L, Buls S, Van Humbeeck J, and Kruth J-P (2013) Lowering thermal gradients in Selective Laser melting by pre-heating the baseplate
14. Ali H, Ma L, Ghadbeigi H, Mumtaz K (2017) In-situ residual stress reduction, martensitic decomposition and mechanical properties en-hancement through high temperature powder bed pre-heating of selective laser melted Ti6Al4V. Mater Sci Eng A 695:211–220 15. Kamath C, El-dasher B, Gallegos GF, King WE, Sisto A (2013)
Density of additively-manufactured, 316L SS parts using laser powder-bed fusion at powers up to 400W. Lawrence Livermore National Laboratory, Livermore
16. Vaithilingam J, Goodridge RD, Hague RJM, Christie SDR, Edmondson S (2016) The effect of laser remelting on the surface chemistry of Ti6al4V components fabricated by selective laser melting. J Mater Process Technol 232:1–8
17. Parry L, Ashcroft IA, Wildman RD (2016) Understanding the effect of laser scan strategy on residual stress in selective laser melting through thermo-mechanical simulation. Addit Manuf 12:1–15 18. Foroozmehr A, Badrossamay M, Foroozmehr E, Golabi I (2016)
Finite element simulation of selective laser melting process consid-ering optical penetration depth of laser in powder bed. Mater Des 89:255–263
19. Roberts IA (2012) Investigation of residual stresses in the laser melting of metal powders in additive layer manufacturing. University of Wolverhampton, Wolverhampton